Dynamic Ferromagnetic Hysteresis Modelling Using
a Preisach-Recurrent Neural Network Model
Christian Grech 1,2,* , Marco Buzio 2 , Mariano Pentella 2,3 and Nicholas Sammut 1,2
1 Faculty of Information and Communications Technology, University of Malta, MSD2080 Msida, Malta;
2 CERN, European Organization for Nuclear Research, 1211 Geneva, Switzerland;
Marco.Buzio@cern.ch (M.B.); firstname.lastname@example.org (M.P.)
3 Department of Applied Science and Technology, Politecnico di Torino, 10129 Turin, Italy
* Correspondence: email@example.com
Received: 10 May 2020; Accepted: 29 May 2020 ; Published: 4 June 2020
Abstract: In this work, a Preisach-recurrent neural network model is proposed to predict the dynamic
hysteresis in ARMCO pure iron, an important soft magnetic material in particle accelerator magnets.
A recurrent neural network coupled with Preisach play operators is proposed, along with a novel
validation method for the identification of the model’s parameters. The proposed model is found
to predict the magnetic flux density of ARMCO pure iron with a Normalised Root Mean Square
Error (NRMSE) better than 0.7%, when trained with just six different hysteresis loops. The model
is evaluated using ramp-rates not used in the training procedure, which shows the ability of the
model to predict data which has not been measured. The results demonstrate that the Preisach model
based on a recurrent neural network can accurately describe ferromagnetic dynamic hysteresis when
trained with a limited amount of data, showing the model’s potential in the field of materials science.
Keywords: ARMCO pure iron; dynamic hysteresis loop; machine learning; magnetic properties;
particle accelerators; Preisach; recurrent neural networks
The phenomenon of hysteresis occurs when a system is not only dependent on present input
values, but also on past input values. The resulting hysteresis loops make modelling a challenge
due to the non-linearity exhibited. In phenomena such as ferromagnetism, dynamic effects add
a further aspect of complexity. The interaction between electric and magnetic fields results in
induced eddy currents, which modify the magnetic hysteresis characteristics. Proposed models
to predict hysteresis can be classified into two main categories: physical models and phenomenological
models. The physical models are built on the description of the object being modelled using
physics laws. Unfortunately, in most cases such models are mathematically complex and require
detailed knowledge of the physical properties of the material being modelled. Phenomenological
models make use of conventional identification methods, which typically have no physical meaning.
Such models are mostly empirical, based on previously acquired experimental data. The most popular
phenomenological hysteresis model is the Preisach model , used in a vast range of applications.
Among the different hysteresis models available in literature, the Preisach-type models prove to have
a great potential to explain various magnetization processes, and is one of the most popular models to
capture the hysteresis behaviour in non-linear systems.
The biggest challenge in implementing a Preisach model is the identification of the model
parameters, because the use of empirical methods makes the procedure problem-dependent .
There are numerous identification methods used in literature [3–5]. In most cases, such a function
Materials 2020, 13, 2561; doi:10.3390/ma13112561 www.mdpi.com/journal/materials
Materials 2020, 13, 2561 2 of 14
can be identified using measured data and applying a numerical approach, which can be a specific
formulation [6,7] or using conventional methods such as an Everett integral  or Gaussian/Lorentzian
functions . The function can then be applied in software using a look-up table of values.
Other ‘black-box’ identification techniques used alongside the Preisach model include genetic
algorithms , fuzzy models  and artificial neural networks (ANN) [12–14]. In , Saliah et al.
showed that using an ANN can match results produced by the conventional methods, considerably
reducing the time overhead. In , Serpico and Visone build an ANN hysteresis model, which is able
to model rate-independent hysteresis when combined with Preisach operators as inputs. Similarly,
different neural network configurations have been used for modelling the rate-independent hysteresis
of magnetic shape memory alloys [17,18].
The Preisach model implementation described above is rate-independent, meaning that the
hysteresis output is determined solely by the input’s extreme values, and the input ramp rates do not
impact the hysteresis loop. Mayergoyz  introduced the dependence of the weight function on the
speed of output variations; similarly, Mrad and Hu  and Song and Li  proposed an input-rate
dependence of the weight function. Both methods suppose the weight function is the right place to
add in dynamic behaviors. On the other hand, in  a linear dynamic model is added before the
classical Preisach operator and the dynamics are assumed to only happen inside the linear dynamic
part. The latter cascade structure can be referred to as an ‘external dynamic hysteresis model’ and is
found in several works [23–25]. In this work, we will consider the rate-dependency without including
an additional element. This can be accounted for by implementing the Preisach model’s weighting
function using dynamic neural networks such as a recurrent neural network (RNN), where each layer
has a recurrent connection, allowing the network to have an infinite dynamic response to time series
input data. An example of the implementation of such model configurations for hysteretic data can be
found in , where an Elman RNN was successful in predicting the major loop at several frequencies.
In , with the addition of Preisach operators at the input stage of an internal time-delay neural
network, the major and minor loop hysteresis of a Giant Magnetostrictive Actuator was modelled
successfully, however this work did not demonstrate functionality in the saturation regions.
In this paper, a Preisach model is implemented using a single RNN, which is able to predict the
different dynamic hysteresis loops of ferromagnetic materials, when a limited amount of measurement
data is available. In particular, the model is trained using three particular frequencies and tested on a
data set which consists of a different frequency. As a novel contribution to the current research state,
both major and minor loop hysteresis are investigated, including saturation regions. The motivation
behind this work lies in the prediction of the dynamic behaviour of materials used in the manufacturing
of magnets for particle accelerators. As an example, ARMCO is used as a test material being used
as part of the superconducting magnets for the High Luminosity upgrade of the Large Hadron
Collider at the European Nuclear Research Centre (CERN) [28,29], where pulsed fields are employed.
Hence, the knowledge of the material’s dynamic behaviour, which is not easily modelled, is required
and this work attempts to propose an accurate model, trained with a limited amount of measurement
data, which can also be used at a moderate computational cost. Whilst a vector hysteresis model
is required for a 3D model of an accelerator magnet, the model can be used to describe the vertical
field used for the RF control of synchrotrons. The description of the eddy-currents transients when
ramping up the material during a test is complicated due to its hysteretic behaviour and the geometry,
generally toroidal, which complicates the formulation . This combined with the intrinsic nature of
the flux-metric method adopted for the material measurement, introduces an uncertainty component
on the results, especially on the coercive field determination [31,32]. The knowledge of the dynamic
behaviour of the material can be potentially used to extrapolate the data in DC, allowing the separation
of the rate-independent hysteresis from the rate-dependent part, and reducing the overall uncertainty.
In Section 2, the experimental details behind the measurements, the theory behind the model and
the validation technique are described. Section 3 describes the results obtained, including the results
of a univariate sensitivity analysis. As test material, ARMCO was considered, being an important
Materials 2020, 13, 2561 3 of 14
yoke material in particle accelerators . Moreover, having an electrical conductivitiy in the order
of 108 S/m and a relative permeability in ther order of 3000, the effect of the eddy currents on the
hysteresis loop can be measured with a good signal-to-noise ratio.
2. Materials and Methods
2.1. Experimental Details
The measurements in this work are performed using a split-coil permeameter , shown in
Figure 1, and performed on toroidal test specimens. The equipment consists of three 90-turn coils,
separable by means of an opening mechanism. A slot allows the insertion of the sample to be tested in
the permeameter, therefore avoiding the time-demanding operation of a custom coil winding onto
the sample . The two outermost coils are used as excitation coils and p